Mathematics and Mechanics of Solids 1–18

Ó The Author(s) 2018 Reprints and permissions:

sagepub.co.uk/journalsPermissions.nav DOI: 10.1177/1081286518773806 journals.sagepub.com/home/mms

### Effect of a rigid toroidal inhomogeneity on

### the elastic properties of a composite

Stanislav Krasnitskii

Petra Velikogo Institut fiziki nanotehnologij i telekommunikacij, Sankt-Peterburgskij politehni-ceskij universitet, St Petersburg, Russia

Anton Trofimov

Center for Design, Manufacturing and Materials, Skolkovo Institute of Science and Technology, Skolkovo, Russia

Enrico Radi

Department of Science and Methods in Engineering, University of Modena and Reggio Emilia, Modena, Italy

Igor Sevestianov

Department of Mechanical and Aerospace Engineering, New Mexico State University, Las Cruces, NM, USA

Received 20 November 2017; accepted 9 April 2018 Abstract

An analytical solution is obtained for the problem of an infinite elastic medium containing a rigid toroidal inhomogeneity under remotely applied uniform strain. The traction on the torus surface is determined as a function of torus parameters and strain components applied at infinity. The results are utilized to calculate components of the stiffness contribution tensor of the rigid toroidal inhomogeneity that is required for calculation of the overall elastic properties of a material containing multiple toroidal inhomogeneities. The analytical results are verified by comparison with finite element model calculations.

Keywords

Rigid torus, stiffness contribution tensor, effective elastic properties, composite, non-ellipsoidal inhomogeneity 1. Introduction

The paper focuses on the problem of a rigid inhomogeneity of toroidal shape embedded in an elastic matrix. Inhomogeneities of this kind occur in both natural and man-made materials. Figure 1 provides several examples. Barium titanate nanotori are used as nonvolatile memory devices, transducers, optical modulators, sensors, and more recently possible energy storage in supercapacitors [1]. Toroidal particles

Corresponding author:

Igor Sevostianov, Department of Mechanical and Aerospace Engineering, New Mexico State University, Las Cruces, NM, USA. Email: [email protected]

represent the preferred morphology of Li2O2deposition on porous carbon electrodes in lithium–oxygen

batteries [2,3]. Polymeric ‘‘microdonuts’’ are used in bioengineering [4]. The toroidal shape of nanoparti-cles is reported to be preferred for microwave absorption properties of BaTiO3 [5]. Onaka et al. [6]

reported the formation of toroidal particles of SiO2in a Cu matrix due to internal oxidation of a Cu–Si

solid-solution polycrystal. Analytical modeling of materials with such microstructure has not been well developed. In the homogenization schemes, the inhomogeneities are usually assumed to be of ellipsoidal shape. This unrealistic assumption is largely responsible for insufficient linkage between methods of micromechanics and materials science applications.

While many analytical and numerical results have been obtained for two-dimensional non-elliptical inhomogeneities [10–13], only a limited number of numerical results and approximate estimates are available for non-ellipsoidal three-dimensional (3D) shapes. Most of them are related to pores and cracks. In the context of compliance of irregularly shaped cracks, certain results have been obtained [14–18]. Various concave pores have also been analyzed [19–22].

For toroidal shapes, Argatov and Sevostianov [23] used asymptotic methods to evaluate the contribu-tion of a thin rigid toroidal inhomogeneity into overall stiffness. Onaka and colleagues [6,24,25] derived analytical expressions for components of the Eshelby tensor for a toroidal inclusion. We emphasize, however, that the Eshelby tensor for non-ellipsoidal inhomogeneities is irrelevant to the problem of effective properties of a heterogeneous material (as clearly seen from the formulation of the two Eshelby problems; see, for example, Chen et al. [21]). The problem on the effective conductivity (thermal or elec-tric) of a material containing toroidal insulating inhomogeneities has been addressed by Radi and Sevostianov [26].

The present work focuses on the evaluation of the contribution provided by a rigid toroidal
inhomo-geneity to effective elastic properties. We first consider a homogeneous elastic material (matrix), with the
stiffness tensor C0assumed to be isotropic. It contains an inhomogeneity, of volume Vð Þ1_{, of a different}

elastic material with the compliance and stiffness tensor C1. The contribution of the inhomogeneity to the overall stress, per representative volume V (the extra stress, as compared to the homogeneous matrix) is given by the fourth-rank tensor N– the stiffness contribution tensor of the inhomogeneity – defined by

Ds = V

1 ð Þ

V N :e

‘ _{ð1Þ}

Figure 1. (a) The morphology of BaTiO3 nanotorus [1]; (b) copolymer bilayer toroidal vesicles have the potential application in biomimicry [7]; (c), (d) polymeric toroidal particles [8], [9]

where e‘_{is the ‘‘remotely applied’’ strain. For a rigid inhomogeneity, this additional stress field Ds can}

be represented as integral over the inhomogeneity boundary [27] D s = 1 V ð S s n ð Þ x dA, ð2Þ

where n is the outward unit normal to the inhomogeneity surface S at point x.

To calculate components of the stiffness contribution tensor of a rigid toroidal inhomogeneity, a dis-placement boundary value problem has to be solved for 3D elastic space containing such and inhomo-geneity. This problem has been addressed previously [28–30]. In the text to follow, we modify the previous solution to calculate the components of the stiffness contribution tensor.

2. Formulation of the problem in toroidal coordinates

We consider a rigid circular torus embedded in an infinite elastic medium subject to remotely applied homogeneous strain field. Following Morse and Feshbach [31] and Lebedev and Silverman [32], we introduce a toroidal coordinate system (a,b,u) (Figure 2) defined by the following relations

x = c sinh a cos u cosh a cos b, y = c sinh a sin u cosh a cos b, z = c sin b cosh a cos b: ð3Þ

where c denotes the distance of the poles from the origin, a . 0, b2 [2p, p], and j2 [0, 2p].

Constant values of the bipolar coordinate a describe a family of toroidal surfaces. R0and r0 denote

medium radius of the torus and the radius of its circular cross-section, respectively. Then a0=cosh1ðR0, r0Þ, c = r0 sinh a0= ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R2 0 r20 q : ð4Þ

Figure 2. Toroidal coordinate system (a, b, j). Associated Cartesian (x, y, z) and cylindrical (r, u, z) coordinate systems are also shown. The coordinate surfaces a0= const are the eccentric family of tori and b0= 6const are spherical caps having there centers

With reference to an arbitrary meridian section, the poloidal angle c2 p, p½ around the circle defined by a constant value of a is associated with the toroidal coordinate b by the following relations:

sin c = sinh a sin b

cosh a cos b and cos c =

cosh a cos b 1

cosh a cos b : ð5Þ

Then a torus surface a = a0can be defined parametrically as follows:

x =(R0+ r0cos c) cos u, y = (R0+ r0cos c) sin u, z = r0sin c: ð6Þ

Let
Pk_{n1=2}(cosha) =G(n + 1=2 + k)
p G(n + 1=2)
ð
p
0

( cosh a + sinh a cos t)n1=2cos kt dt, ð7Þ

Qk_{n1=2}( cosh a) = ( 1)
k
2pﬃﬃﬃﬃﬃﬃ2p G(k + 1=2) sinh
k
a
ðp
p
cos nt
( cosh a cos t)k + 1=2 dt, ð8Þ
denote the associated Legendre function of semi-integer index and order k of the first or the second kind,
respectively [32–34]. They satisfy the following equations

DkPk_{n1=2}( cosh a) = 0, DkQk_{n1=2}( cosh a) = 0, ð9Þ

where the operator Dk is defined by

Dk = ∂2 ∂r2 + 1 r ∂ ∂r + ∂2 ∂z2 k r2: ð10Þ

3. Analytical solution for a rigid toroidal inclusion in an infinite elastic medium

The total displacement field u in the infinite elastic medium containing a rigid toroidal inclusion can be
represented as a sum u = u‘+ u0where u‘corresponds to the remotely applied homogeneous strain field
and u0_{is the correction due to the presence of the toroidal inhomogeneity. Due to the geometrical }

sym-metry of the problem, the stiffness contribution tensor N is expected to be transversely isotropic. Therefore, it is sufficient to consider the following Cartesian components of the remotely applied strains: e‘

zz, e ‘

yy, and e ‘

yz. Then, the fundamental displacement field admits the following Cartesian

components

u‘_{x} = 0
u‘_{y} =e‘_{yy}y

u‘_{z} = 2e‘_{yz}y + e‘_{zz}z

ð11Þ

The corresponding displacement components in cylindrical coordinates can be written as
u‘r =
1
2e
‘
yyr
1
2e
‘
yyr cos 2u
u‘_{f}=1
2e
‘
yyr sin 2u
u‘_{z} =e‘_{zz}z + 2e‘_{yz}r sin u
ð12Þ

For the general case of arbitrary load, the inhomogeneity may be subjected to rigid body translation and rotation. In this case the boundary conditions on the inhomogeneity surface could be represented in the form of the Robin problem [34] as u = d + v× x, where d and v are vectors of small translation and rotation of the rigid inhomogeneity, and x is a position vector on the interface. In the case of tensile strain e‘

zz and e‘yy, the rigid motion of the torus can be ignored due to the symmetry of the applied loads

and geometry. In contrast, simple shear deformation e‘

yz leads to the rigid rotation of the toroid with

respect to its center with d = 0 and v = v ex, where v is the rotation angle of the torus (to be determined)

and ex is a unit vector along the x-axis. Then, in the cylindrical coordinate system,

u_{r}= v z sin u
u_{u}= v z cos u

u_{z}= v r sin u ð13Þ

In the study by Krokhmal [35], it was suggested to seek for the corrective term u0_{in the following form}

u0_{r}=1
2u
0
0(a, b) + u
0
2(a, b) cos 2u
u0_{u}= v0_{2}(a, b) sin 2u
u0_{z} =1
2w
0
0(a, b) + w
0
1(a, b) sin u ð14Þ
where
u0_{0}= f1+ grq0, w00= x0+ gzq0, w01= x1+ gzq1
u0_{2}= f3+ c1+ grq2, v02= f3 c1
ð15Þ
g = 1=½4 (1 n), and the functions qk, fk, ck, and xksatisfy the following relations

Dkqk= 0, Dk + 1fk + 1= 0, Dk1ck1= 0, Dkxk= 0, ð16Þ

and the differential constraint
g 1 + 1
g + r
∂
∂r + z
∂
∂z
qk+
∂
∂r +
k + 1
r
fk + 1+
∂
∂r
k 1
r
c_{k1}+ ∂
∂zxk= 0, kð 0Þ ð17Þ
with c21= 0.

The general solutions to equations (16) matching the displacement field of equations (12) and (13) have the following form

qk=
1
c
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
cosh a cos b
p X+ ‘
n = 0
0_{A}
n, kPk_{n1=2}( cosh a) cos (nb k2p=2)
fk=
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
cosh a cos b
p X+ ‘
n = 0
0_{B}
n, kPk + 1_{n1=2}( cosh a) cos (nb k2p=2)
c_{k}=pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃcosh a cos b X
+ ‘
n = 0
0_{D}
n, kPk1_{n1=2}( cosh a) cos (nb k2p=2)

x_{k}=pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃcosh a cos b X

+ ‘

n = 0
0_{C}

n, kPkn1=2( cosh a) sin (nb k2p=2) ð18Þ

for k = 0, 1, 2, 3. The primed summation in equation (18) denotes that the first term of the sum corre-sponding to n = 0 is halved.

The unknown coefficients An,k, Bn,k, Cn,k, and Dn,k can be determined from the boundary condition

at a = a0, together with the differential constraint (equation (17)). By using equations (11)–(14), the

boundary conditions at a = a0require

u0_{0}(a0, b) = e‘yyrja = a0 u
0
1(a0, b) = v zja = a0 u
0
2(a0, b) =
1
2e
‘
yyrja = a0
v0_{1}(a0, b) = v zja = a0 v2(a0, b) =
1
2e
‘
yyrja = a0
w0_{0}(a0, b) = 2e‘zzzja = a0 w
0
1(a0, b) = (v 2e‘yz) rja = a0 ð19Þ

Introducing the unknowns xn,kfor the coefficients Bn,kand using equations (15) and (19), all the

coef-ficients in the Fourier series of equation (18) can be written in terms of xn,kas follows

A0, k= ß0, kð2x1, k 2 cosh a0x0, k+ p0, kÞ=g,
An, k= ßn, kðxn + 1, k 2 cosh a0xn, k+ xn1, k+ pn, kÞ=g, n 1ð Þ
Bn, k= ln, kxn, k, nð 0Þ
C0, 0= 0,
C0, 1= ß0, 1ðs0, 1 2 x1, 1Þ,
Cn, k= ßn, kðxn1, k xn + 1, k+ sn, kÞ, n 1ð Þ
Dn, k= gn, kðxn, k+ qn, kÞ, n 0ð Þ ð20Þ
where
ßn, k=
dk
sinh a0Pk_{n1=2}( cosh a0)
, g_{n, k}= ek
Pk1_{n1=2}( cosh a0)
, ln, k=
1
Pk + 1_{n1=2}( cosh a0)
, ð21Þ

being d0= 1/2, e0= 0, and dk= ek= 1, for k 1. Coefficients pn,k, qn,k, and sn,kare the Fourier

coeffi-cients for the following functions
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
cosh a0 cos b
p
(u0k+ekv0k) = dk
X+ ‘
n = 0
0_{p}
n, kcos(nb k2p=2),
ek v
0
k
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
cosh a0 cos b
p =ek
X+ ‘
n = 0
0_{q}
n, k cos(nb k2p=2), ð22Þ
w0_{k}sinh a_{ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ}0 (u0k+ekv0k) sin b
cosh a0 cos b
p = dk
X+ ‘
n = 0
0_{s}
n, k sin(nb k2p=2),

Using the decomposition given in the Appendix, we finally obtain the following relations pn, 0=

4pﬃﬃﬃ2 p e

‘

qn, 1= 0
sn, 0=
8pﬃﬃﬃ2
p (e
‘
yy 2e
‘
zz)c sinh a0n Qn1=2( cosh a0)
pn, 1= 0
qn, 1=
4pﬃﬃﬃ2
p v c n Qn1=2( cosh a0)
sn, 1=
4pﬃﬃﬃ2
p (v 2e
‘
yz)c sinh a0Q1_{n1=2}( cosh a0)
pn, 2= 0
qn, 2=
2pﬃﬃﬃ2
p e
‘
yyc sinh a0Q1n1=2( cosh a0)
sn, 2= 0
ð23Þ

and obtain the following infinite system of algebraic equations for the unknown variables xn,k:

an, kxn + 1, k bn, kxn, k+ cn, kxn1, k= dn, k, ð24Þ
where
an, k= 2(n + k + dn)ßn + 1, kcosh a0+(2n + 1 + 2=g)ßn, k n + k + 1=2ð Þ n + k + 3=2ð Þln + 1, k gn + 1, k,
bn, k= 2 n + k + 1=2ð Þßn + 1, k+2dn(1 + 2=g)ßn, kcosh a0+2en(n k 1=2)ßn1, k
2 n + k + 1=2ð Þ(n k 1=2)ln, k 2dngn, k,
cn, k=en½2(n k 1=2)ßn1, kcosh a0 (2n 1 2=g)ßn, k (n k 1=2)(n k 3=2)ln1, k gn1, k,
dn, k= g_{n + 1, k} qn + 1, k 2dngn, k qn, k+eng_{n1, k} qn1, k n + k + 1=2ð Þßn + 1, k(pn + 1, k+ sn + 1, k)
dn(1 + 2=g)ßn, k pn, k+en(n k 1=2)ßn1, k(pn1, k sn1, k) + en 2n ßn, ksn, k,
ð25Þ
for n 0. Note that for k = 0, 2 equation (25) holds for n 0, while for k = 1 it holds for n 1.

A necessary condition for the series in equation (18) to be convergent is that the coefficients An,k, Bn,k,

Cn,kand Dn,ktend to zero as n! ‘. Thus, the unknown coefficients xn,khave to converge to zero. In this

case, the infinite system of equations (24) can be solved explicitly using the procedure for tridiagonal
matrix
xn=
X+ ‘
m = n
h_{m + 1} Y
m
k = n + 1
jk ð26Þ
where
jn + 1=
an
bn cnjn
, hn + 1=
cnhn dn
bn cnjn
:
From the conditions for n = 0 and k = 0, 2

j1= a0 b0 , h1= d0 b0 : From the conditions for n = 0 and k = 1

Once the unknown coefficients xn,k have been determined, the total displacement field in cylindrical

coordinates is given by the sum of equations (12), (13), and (14). Then, the corresponding strain field can be calculated from the compatibility condition:

err= ∂ur ∂r , ejj= 1 r ∂uj ∂j + ur r , ezz= ∂uz ∂z , erj= 1 2 1 r ∂ur ∂j + ∂uj ∂r uj r , erz= 1 2 ∂ur ∂z + ∂uz ∂r , ejz= 1 2 1 r ∂uz ∂j + ∂uj ∂z , ð27Þ

where we used connection between derivatives in cylindrical and toroidal coordinate systems ∂

∂r = 1

c ( cosh a cos b 1) ∂

∂a+sinh a sin b ∂ ∂b , ∂ ∂z = 1 c sinh a sin b ∂

∂a +( cosh a cos b 1) ∂ ∂b

, ð28Þ

and expressions for derivatives of the associated Legendre functions given in the Appendix. Finally, the stress field is obtained from the Hooke’s law

s = E 1 + n e + n 1 2n tr e I , ð29Þ

where E and n are the Young’s modulus and Poisson ratio of the isotropic matrix and I is the second-rank unit tensor.

The Cartesian components of the stress tensor s can be easily expressed via cylindrical components sxx= srrcos2u + suusin2u 2srusinu cosu,

syy= srrsin2u + suucos2u 2srusinu cosu,

sxy= sru cos2u sin2u + srr suu sinu cosu, sxz= szrcosu szusin u, syz= szrsinu szucos u: ð30Þ

The traction vector at the torus surface a = a0is t =2ea s with the outer unit normal

n = 1

cosh a0 cos b

(cosh a0cos b 1) cos j, (cosh a0cos b 1) sin j, sinh a0sin b

f g, ð31Þ

The principal moment produced by torus surface tractions is M = ð s t× x dA ð32Þ where x = c cosh a0 cos b

fsinh a0 cos u, sinh a0 sin u, sin bg ð33Þ

is the position-vector of a point on the torus surface. The infinitesimal element of torus surface is given as [31]

dA = c

2_{sinh a}
0

(cosh a0 cos b)2

dudb: ð34Þ

The solution obtained of the boundary value problem for an elastic medium with rigid torus is speci-fied below for three load cases: e‘

zz, e ‘ yy and e

‘ yz.

(i) Tension along z-axis. The nonzero component of remote elastic strain is e‘

zz. In this case the total

displacement field has axial symmetry about the z-axis and vanishes on the surface of the torus. The maps for the displacement components uyand uz are shown in Figure 3 for the meridional

cross-section of the matrix near the inhomogeneity.

The distribution of Cartesian component of stress vector on the torus surface (a = a0) is shown in

Figure 4.

(ii) Tension along y-axis. The nonzero component of remote elastic strain is e‘

yy. The total

displace-ment vanishes on the surface of the rigid toroidal inclusion. The distribution of the displacedisplace-ment components uy and uz is illustrated in Figure 5 for the meridional cross-section of the matrix

near the inhomogeneity. The distribution of Cartesian component of stress vector on the torus surface (a = a0) is shown in Figure 6. It is seen that the boundary condition are satisfied on rigid

torus surface for both (i) and (ii) load cases.

(iii) Simple shear in yz plane. The nonzero component of remote elastic strain is e‘

yz. Under shear,

the toroidal inhomogeneity has rigid rotation on angle v to be determined from the moment equilibrium condition with respect to the inhomogeneity

Mv+ Mg= 0 ð35Þ

where Mvis resultant moment required to produce rotation on angle v and Mgis the reactive moment

caused by simple shear e‘

yz. Moments could be calculated using the equation (32)

Mv= ð S t(e‘yz= 0)× x dA My= ð S t(v = 0)× x dA ð36Þ

Figure 3. The distribution of the (a) ux= uyand (b) uzdisplacement components near rigid toroidal inhomogeneity (R0/r0= 2) in

infinite media under tension along the z-axis, i.e. for e‘

zz= 1 and e‘yy= g‘yz= 0. The maps are plotted for a meridian plane y = 0. The displacement values are given in units of R0for n = 0.3.

Due to the linearity of the problem, forces and moments are proportional to the displacements and rotations, respectively. Then, accounting for the equilibrium equation (34), the rotation angle can be cal-culated as v = 2 Mg Mv e‘yz ð37Þ

The dependence of v on the aspect ratio of torus is shown in Figure 7.

The distribution of the displacement components uyand uzunder simple shear e‘yzis shown in Figure 8

for the meridional cross-section of the matrix near the torus.

The distribution of Cartesian component of the traction vector on torus surface is shown in Figure 9. We now can calculate the components of the stiffness contribution tensor N for a rigid toroidal inhomo-geneity using equations (1) and (2), namely

N : e‘= 1 V

ð

s

tx dA, ð38Þ

where V= 2p2r_{0}2R0 is the volume of the torus and dA is the infinitesimal element of torus surface (see

equation (34)). In the toroidal coordinate system traction t and position vector x is given by equations (29)–(31) and (34). Then the normalized dependence of the stiffness contribution tensor N on torus aspect ratio l = r0/R0can be obtained from equation (38).

Figure 4. The distribution of the (a) tx, (b) ty, and (c) tztraction components at the torus surface a = a0, R0/ r0= 2 with respect to

azimuth u and poloidal angel c. The nonzero component of remote strain is e‘

zz= 1. The stress values are given in units of E for n = 0.3.

4. Finite element model

To verify the analytical solution, we also calculate components of the stiffness contribution tensors using finite element analysis (FEA). To produce the necessary 3D mesh of the considered shape we start by generating surface mesh in a custom MATLAB script [36,37]. A torus surface is defined parametrically using equation (6). Since the coordinates are stored in the form of an ordered list they can easily be con-nected into the continuous mesh with triangular elements. Note that each mesh generated using our script is composed of approximately 30,000 surface elements (see Figure 10).

Torus surface mesh is then placed into a large reference volume V that has cubic shape with sides at least five times bigger than the largest linear dimension of the inhomogeneity to reduce boundary effects and simulate remote loading. This setup is auto meshed with non-linear tetrahedral 3D elements due to higher accuracy of results compared to linear elements. An example of the mesh is given in Figure 11. To simulate perfectly rigid inhomogeneity we assume that the ratio of matrix and inhomogeneity Young’s moduli is Ei/E =1010. The boundary ∂V of the reference volume I is subject to the kinematic

conditions

uj_{∂V}= e‘ x ð39Þ

At the next step, to find all nonzero components of tensor N we perform a set of six load cases in FEA package MSC Marc Mentat: three normal loadings in the directions of three global coordinate axes and three shear loads according to equation (39). Once the numerical simulations are completed for the given shape, the result files are processed to calculate all volume-averaged stress components within V from each load case:

Figure 5. The distribution of the (a) ux, (b) uy, and (c, d) uzdisplacement components near rigid toroidal inhomogeneity (R0/ r0= 2)

in infinite media under tension along the y-axis, i.e. for e‘

yy= 1 and e‘zz= g‘yz= 0. The maps are plotted for the meridian planes: (a) and (c) for y = 0; (b) and (d) for x = 0. The displacement values are given in units of R0for n = 0.3.

sij
m=
1
V
XNe
l = 1
(s(l)ij )_{m}V
(l)_{ð}_{i, j = 1, 2, 3; m = 1, 2, :::, 6}_{Þ} _{ð40Þ}
where sij

m is the volume average of the stress component ij calculated from the mth load case, V is

the reference volume,(s(l)ij )m is the stress component ij at the centroid of the finite element l calculated Figure 6. The distribution of the (a) tx, (b) tyand (c) tztraction components at the torus surface a = a0, R0/ r0= 2 with respect to

azimuth u and poloidal angel c. The nonzero component of remote strain is e‘_{yy}= 1. The stress values are given in units of E for
n = 0.3.

Figure 7. Dependences of rotation angle v of inclusion with respect to torus aspect ratio r0/R0for g‘_{yz}= 1 and different values of

from the mth load case, V(l)is the volume of the element l, and Ne is the total number of elements in

the model.

Figure 8. The distribution of the (a) uyand (b) uzdisplacement components near rigid toroidal inhomogeneity (R0/r0= 2) in infinite

media under simple shear in the yz plane, i.e. for g‘

yz= 1, v ’ 0.794, and e‘yy=e‘zz= 0. The maps are plotted for the meridian plane x = 0. The displacement values are given in units of R0for n = 0.3.

Figure 9. The distribution of the (a) tx, (b) ty, and (c) tztraction components at the torus surface a = a0, R0/ r0= 2 with respect to

azimuth u and poloidal angel c. The nonzero component of remote strain is g‘_{yz}= 1. The stress values are given in units of E for
n = 0.3.

Given the average stress components we then calculate the stiffness contribution tensor from:
Nijkl(e‘_{kl})m= sij
m (s
‘
)mðsummation over k, l = 1, 2, 3Þ ð41Þ
where(e‘

kl)mare the components of the prescribed strain and(s‘ij)m are the stress components inside V in

the absence of the inhomogeneity. Components of the stiffness contribution tensors are than normalized
by particle volume fraction and matrix Young’s modulus E as follows, Nijkl=_{EV}VNijkl, where V*is torus

inhomogeneity volume. Figure 12 illustrates comparison of the nonzero components of stiffness contri-bution tensor calculated analytically using equation (38) with ones obtained by FEA.

5. Approximation by spheroid

We now compare the obtained results with ones for stiffness contribution tensor of an oblate rigid spher-oid of the aspect ratio x components of this tensor can be written as follows:

N1111= p6 4 p1p6 p23 + 1 2p2 , N1122= p6 4 p1p6 p23 1 2p2 , N1212= 1 2p2 , N3333= p6 p1p6 p23 ; N1133= p3 2 p1p6 p23 , N1313= 1 p5 , where

Figure 10. Torus surface meshes for different ratio r0/R0(a) 0.5 and (b) 0.3.

Figure 11. Example of a mesh density of the matrix and torus with r0/R0= 0.5: (a) general view; (b) close-up view of the highlighted

p1= 1 2m½(1 k)f0+ k f1; p2= 1 2m½(2 k)f0+ k f1, p3= p4= k f1 m , p5= 1 m½1 f0 4kf1, p6= 1 m½(1 k)(1 2f0) + 2k f1: ð42Þ

and the following notation is used:

m = E
2(1 + n), k =
1
2(1 n), f0=
x2(1 g)
2(x2_{ 1)}, f1=
x2
4(x2_{ 1)}½(2x
2
+ 1)g 3,
g =
1
xpﬃﬃﬃﬃﬃﬃﬃﬃ1x2arctan
ﬃﬃﬃﬃﬃﬃﬃﬃ
1x2
p
x , oblateshape x\1ð Þ
1
2xpﬃﬃﬃﬃﬃﬃﬃﬃx2_{1}ln
x +pﬃﬃﬃﬃﬃﬃﬃﬃx2_{1}
xpﬃﬃﬃﬃﬃﬃﬃﬃx2_{1}, prolateshape x . 1ð Þ
8
>
<
>
: ð43Þ

Argatov and Sevostianov [23], using asymptotic methods, showed that in-plane components of the stiffness contribution tensor of a thin rigid torus can be approximated with good accuracy by the corre-sponding components calculated for a rigid spheroid that has the same radius and the same volume. For an oblate spheroid, it gives the aspect ratio of the spheroid in terms of the aspect ratio of the torus l = r0=R0as follows:

Figure 12. Normalized nonzero components of the stiffness contribution tensor of inhomogeneity (a) N1111= N2222, (b) N3333, (c)

N1122, (d) N1133, (e) N1212, and (f) N1313= N2323as function of the aspect ratio r0/R0. The solid curves correspond to the rigid

toroidal inclusion; The dashed curves correspond to the rigid ellipsoidal inclusion; the FEM results are noted by marks. The stiffness values are given in units of eijE for different values of Poisson ratio 0.0, 0.3, and 0.45.

x = 3p l

2

2(1 + l)3: ð44Þ

Equation (44) gives us a spheroid that has the same volume and the same radius as the torus. These com-ponents are shown in Figure 12(a), (c), and (e) as functions of l.

Out-of-plane components of the stiffness contribution tensor of a rigid torus can be approximated by the in-plane components of a rigid prolate spheroid that has the same radius and the same volume. In this case, to preserve the radius and the volume, the aspect ratio of the spheroid has to be

x = 3p

2l ð55Þ

Figure 12(b), (d), and (f) illustrate a comparison between the components of the stiffness contribution tensors for rigid inhomogeneities of toroidal and prolate spheroidal pores. It is seen that the lines are quite close to each other with the exception of N1313.

6. Discussion and conclusions

We solved an elasticity boundary-value problem for an infinite elastic medium containing a rigid toroi-dal inhomogeneity subjected to remotely applied uniform strains. The solution is obtained in explicit form of associated Legendre function’s series using the approach proposed by Eroshkin and Tsukrov [27]. Displacement and traction is determined as a function of coordinates, torus parameters and strain components applied at infinity. We managed to combine the procedures for solving the axisymmetric (k = 0) and asymmetric (k 1) case and write the solution in the most general form. The boundary-value problems were reduced to infinite systems of algebraic equations with three-diagonal matrices. We suc-ceeded in extending the classical method of solving finite algebraic equations with a tridiagonal matrix to the case of an infinite number of equations.

Considering the toroidal inhomogeneity subject to simple shear in the meridional plane, we have taken into account the rigid rotation of the inhomogeneity. The angle of rotation can be calculated from the equation of moment equilibrium. The angle decreases when the torus aspect ratio increases.

The obtained solution is used to get explicit expressions for the components of stiffness contribution tensor of the rigid toroidal inhomogeneity. The results are verified by comparison with finite element simulating. The components of the stiffness contribution tensor for a torus are compared with ones for a rigid spheroid having the same radius and the same volume as torus. It is shown that the components of the stiffness contribution tensor for an oblate spheroid serve as good approximations for correspond-ing in-plane components of the torus while two out-plane components can be approximated by compo-nents of the stiffness contribution tensor for a prolate spheroid.

The expression for stiffness contribution tensor yields the possibility to calculate effective elastic prop-erties of a material containing multiple toroidal inhomogeneities. Indeed, if interaction between the inhomogeneities is neglected, each inhomogeneity can be assumed to be subjected to the same remotely applied strain, their contributions into the change in the stiffness tensor can be treated separately. In none interaction approximation the extra stiffness due to inhomogeneities of the same shape can always be represented in the form

DC = 1
V
X
iViN
i
ð Þ _{ð56Þ}

where summation over inhomogeneities may be replaced by integration over their orientation. The non-interaction approximation, in turn, serves as the basic building block for various homogenization schemes – self-consistent, differential, Mori–Tanaka, Maxwell, etc. [38].

Funding

References

[1] Bogicevic, C, Thorner, G, Karolak, F, et al. Morphogenesis mechanisms in the solvothermal synthesis of BaTiO3from

titanate nanorods and nanotubes. Nanoscale 2013; 7: 3594–3603.

[2] Horstmann, B, Gallant, B, Mitchell, R, et al. Rate-dependent morphology of Li2O2growth in Li–O2batteries. J Phys

Chem Lett2013; 4: 4217–4222.

[3] Chen, Y, Freunberger, SA, Peng, Z, et al. Charging a Li–O2battery using a redox mediator. Nat Chem 2013; 5: 489–494.

[4] Alexander, L, Dhaliwal, K, Simpson, J, et al. Dunking doughnuts into cells—selective cellular translocation and in vivo analysis of polymeric micro-doughnuts. Chem Commun 2008: 3507–3509.

[5] Xia, F, Liu, J, Gu, D, et al. Microwave absorption enhancement and electron microscopy characterization of BaTiO3

nano-torus. Nanoscale 2011; 3: 3860–3867.

[6] Onaka, S, Sato, H, and Kato, M. Elastic states of doughnut-like inclusions with uniform eigenstrains treated by averaged Eshelby tensors. Philos Mag Lett 2002; 82: 1–7.

[7] Palanisamy, A, and Guo, Q. Giant tubular and toroidal vesicles from self-assembled triblock copolymer–polyaniline complexes in water. Chem Commun 2015: 11100–11103.

[8] Haridas, V, Sapala, AR, and Jasinski, JP. Self-assembling triazolophanes: from croissants through donuts to spherical vesicles. Chem Commun 2015; 6905–6908.

[9] Park, CH, Chung, N, and Lee, J. Monodisperse red blood cell-like particles via consolidation of charged droplets. J Colloid Interface Sci2011; 361: 423–428.

[10] Zimmerman, RW. Compressibility of two-dimensional cavities of various shapes. J Appl Mech 1986; 53: 500–504. [11] Kachanov, M, Tsukrov, I, and Shafiro, B. Effective moduli of solids with cavities of various shapes. Appl Mech Rev 1994;

47: S151–S174.

[12] Tsukrov, I, and Novak, J. Effective elastic properties of solids with defects of irregular shapes. Int J Solids Struct 2002; 39: 1539–1555.

[13] Tsukrov, I, and Novak, J. Effective elastic properties of solids with two-dimensional inclusions of irregular shapes. Int J Solids Struct2004; 41: 6905–6924.

[14] Fabrikant, VI. Applications of potential theory in mechanics: a selection of new results. Dordrecht, the Netherlands: Kluwer Academic Publishers, 1989.

[15] Sevostianov, I, and Kachanov, M. On elastic compliances of irregularly shaped cracks. Int J Fract 2002; 114: 245–257. [16] Grechka, V, Vasconcelos, I, and Kachanov, M. The influence of crack shape on the effective elasticity of fractured rocks.

Geophysics2006; 71: D153–D160.

[17] Mear, ME, Sevostianov, I, and Kachanov, M. Elastic compliances of non-flat cracks. Int J Solids Struct 2007; 44: 6412–6427.

[18] Kachanov, M, and Sevostianov, I. Rice’s Internal variables formalism and its implications for the elastic and conductive properties of cracked materials, and for the attempts to relate strength to stiffness. J Appl Mech 2012; 79: 031002.

[19] Sevostianov, I, Kachanov, M, and Zohdi, T. On computation of the compliance and stiffness contribution tensors of non ellipsoidal inhomogeneities. Int J Solids Struct 2008; 45: 4375–4383.

[20] Sevostianov, I, and Giraud, A. On the compliance contribution tensor for a concave superspherical pore. Int J Fract 2012; 177: 199–206.

[21] Chen, F, Sevostianov, I, Giraud, A, et al. Evaluation of the effective elastic and conductive properties of a material containing concave pores. Int J Eng Sci 2015; 97: 60–68.

[22] Sevostianov, I, Chen, F, Giraud, A, et al. Compliance and resistivity contribution tensors of axisymmetric concave pores. Int J Eng Sci2016; 101: 14–28.

[23] Argatov, I, and Sevostianov, I. Rigid toroidal inhomogeneity in an elastic medium. Int J Eng Sci 2011; 49: 61–74.

[24] Onaka, S, Kobayashi, N, Fujii, T, et al. Energy analysis with a superspherical shape approximation on the spherical to cubical shape transitions of coherent precipitates in cubic materials. Mater Sci Eng A 2003; 347: 42–49.

[25] Onaka, S. Strain fields caused by doughnut-like and tubular inclusions with uniform eigenstrains. Mech Res Commun 2005; 32: 316–322.

[26] Radi, E, and Sevostianov, I. Toroidal insulating inhomogeneity in an infinite space and related problems. Proc R Soc Lond A2016; 472: 20150781.

[27] Eroshkin, O, and Tsukrov, I. On micromechanical modeling of particulate composites with inclusions of various shapes. Int J Solids Struct2005; 42: 409–427.

[28] Solovie, v YI. The axisymmetric problem of elasticity for a torus and a space with toroidal cave. Mekh Tverd Tela 1969: 99–105.

[29] Podil’chuk, YN, and Kirilyuk, VS. Nonaxially symmetric deformation of a torus. Sov Appl Mech 1983; 119: 743–748. [30] Kirilyuk, VS. Stress concentration in an isotropic medium with an elastic toroidal inhomogeneity. Sov Appl Mech 1988; 24:

11–14.

[31] Morse, PM, and Feshback, H. Methods of theoretical physics. New York: McGraw-Hill, 1953.

[33] Hobson, EW. Spherical and ellipsoidal harmonics. Cambridge: Cambridge University Press., 1931. [34] Bateman, H, and Erdelyi, A. Higher transcendental functions. New York: McGraw-Hill, 1953.

[35] Krokhmal, PA. Exact solution of the displacement boundary-value problem of elasticity for a torus. J Eng Math 2002; 44: 345–368.

[36] Trofimov, A, Drach, B, Kachanov, M, et al. Effect of a partial contact between the crack faces on its contribution to overall material compliance and resistivity. Int J Solids Struct. Epub ahead of print 1 March 2017. DOI: 10.1016/ j.ijsolstr.2016.12.028.

[37] Trofimov, A, Drach, B, and Sevostianov, I. Effective elastic properties of composites with particles of polyhedral shapes. Int J Solids Struct2017; 120: 157–170.

[38] Sevostianov, I, and Kachanov, M. Non-interaction approximation in the problem of effective properties. In: Kachanov, M, and Sevostianov, I (eds.) Effective properties of heterogeneous materials, Springer Science & Business Media, 2013, 1– 95.

Appendix Legendre functions

The following recursive relations hold for the function Pk n1=2:

P1_{n1=2}( cosh a) =n + 1=2

sinh a ½Pn + 1=2( cosh a) cosh a Pn1=2( cosh a),
P2_{n1=2}( cosh a) = (n2 1=4) P_{n1=2}( cosh a) 2 coth a P1

n1=2( cosh a),

P3_{n1=2}( cosh a) = (n2_{ 9=4) P}1

n1=2( cosh a) 4 coth a P 2

n1=2( cosh a):

By using the recursive properties of Legendre functions [35] one may obtain d

daPn1=2( cosh a) =

1 + 2n 2 sinh a0

½Pn + 1=2( cosh a) cosh a Pn1=2( cosh a), ðÞ

d
daP
k
n1=2( cosh a) = n2 k
1
2
2
" #
Pk1_{n1=2}( cosh a) k coth a Pk
n1=2( cosh a), kð 1Þ

and similar relations hold for Q_{n1=2}.

The following useful definite integrals involving the Legendre functions and associate Legendre func-tions of first and second kind, denoted as Pk

n1=2 and Q k

n1=2, respectively, have been used in the present

work: ð p p sin b sin nb db (cosh a cos b)3=2= 4pﬃﬃﬃ2 n Qn1=2ðcosh aÞ, ðA1Þ ðp p cos nb db (cosh a cos b)3=2= 4pﬃﬃﬃ2 sinh aQ 1 n1=2ðcosh aÞ, ðA2Þ